- Induction hardening
Induction hardening is a form of
heat treatmentin which a metal part is heated by induction heatingand then quenched. The quenched metal undergoes a martensitic transformation, increasing the hardness and brittleness of the part. Induction hardening is used to selectively harden areas of a part or assembly without affecting the properties of the part as a whole.
Induction heating is a non contact heating process which utilises the principle of
electromagneticinduction to produce heat the surface layer of a work-piece. By placing a conductivematerial into a strong alternating magnetic fieldelectrical current can be made to flow in the steel thereby creating heat due to the I²R losses in the material. In magnetic materials, further heat is generated below the curie pointdue to hysteresislosses. The current generated flows predominantly in the surface layer, the depth of this layer being dictated by the frequency of the alternating field, the surface power density, the permeabilityof the material, the heat time and the diameter of the bar or material thickness. By quenchingthis heated layer in water, oil or a polymerbased quench the surface layer is altered to form a martensitic structure which is harder than the base metal.
A widely used process for the surface hardening of steel. The components are heated by means of an alternating magnetic field to a
temperaturewithin or above the transformation range followed by immediate quenching. The core of the component remains unaffected by the treatment and its physical properties are those of the bar from which it was machined, whilst the hardness of the case can be within the range 37/58 HRC. Carbonand alloy steels with an equivalent carbon contentin the range 0.40/0.45% are most suitable for this process.
A source of high frequency electricity is used to drive a large alternating current through a coil. The passage of current through this coil generates a very intense and rapidly changing magnetic field in the space within the work coil. The workpiece to be heated is placed within this intense alternating magnetic field where eddy currents are generated within the workpiece and resistance leads to
Jouleheating of the metal. This operation is most commonly used in steel alloys. Many mechanical parts, such as shafts, gears, springs, etc. are subjected to surface treatments, before the delivering, in order to improve wear behavior. The effectiveness of these treatments depends both on surface materials properties modification and on the introduction of residual stress. Among these treatments, induction hardening is one of the most widely employed to improve component durability. It determines in the work-piece a tough core with tensile residual stresses and a hard surface layer with compressive stress, which have proved to be very effective in extending the component fatiguelife and wear resistance.
Induction surface hardened low alloyed medium carbon steels are widely used for critical automotive and machine applications which require high wear resistance. Wear resistance behavior of induction hardened parts depends on hardening depth and the magnitude and distribution of residual compressive stress in the surface layer.
The basis of all induction heating systems was discovered in 1831 by
Michael Faraday. Faraday proved that by winding two coils of wire around a common magnetic core it was possible to create a momentary EMFin the second winding by switching the electric currentin the first winding on and off. He further observed that if the current was kept constant, no EMF was induced in the second winding and that this current flowed in opposite directions subject to whether the current was increasing or decreasing in the circuit.
Faraday concluded that an
electric currentcan be produced by a changing magnetic field. As there was no physical connection between the primary and secondary windings the EMF in the secondary coil was said to be induced and so Faraday's law of inductionwas born. Once discovered these principles were employed over the next century or so in the design of electric motor, electrical generatorand forms of electrical transformerand any heat generated in either the electrical or magnetic circuits was felt to be undesirable. Engineers went to great lengths and utilised laminatedcores and other methods to minimise the effects.
Early last century the principals were explored as a means to melt steel and the motor generator was developed to provide the power required for the
induction furnace. After general acceptance of the methodology for melting steel, engineers began to explore other possibilities for the utilisation of the process. It was already understood that the depth of current penetration in steel was a function of its magnetic Permeability (electromagnetism), resistivity and the frequency of the applied field. Engineers at Midvale Steeland The Ohio Crankshaft Company drew on this knowledge to develop the first surface hardening induction heating systems using motor generators.
The need for rapid easily
automatedsystems led to massive advances in the understanding and utilisation of the induction hardening process and by the late 1950s many systems utilising motor generators and Thermionic emission triodeoscillators were in regular use in a vast array of industries. Modern day induction heating units utilise the latest in semiconductor technology and digital control systems to develop a range of powers from 1Kw to many megawatts.
ingle shot hardening
In single shot systems the component is held statically or rotated in the coil and the whole area to be treated is heated simultaneously for a pre set time followed by either a flood quench or a drop quench system. Single shot is often used in cases where no other method will achieve the desired result for example for flat face hardening of hammers, edge hardening complex shaped tools or the production of small gears.
In the case of shaft hardening a further advantage of the single shot methodology is the production time compared with progressive traverse hardening methods. In addition the ability to use coils which can create longitudinal current flow in the component rather than diametric flow can be an advantage with certain complex
There are disadvantages with the single shot approach. The coil design can be an extremely complex and involved process. Often the use of
ferriteor laminated loading materials is required to influence the magnetic field concentrations in given areas thereby to refine the heat pattern produced. Another drawback is that much more power is required due to the increased surface area being heated compared with a traverse approach.
In traverse hardening systems the work piece is passed through the
induction coilprogressively and a following quench spray or ring is utilised. Traverse hardening is used extensively in the production of shaft type components such as axle shafts, excavator bucket pins, steering components, power tool shafts and drive shafts. The component is fed through a ring type inductor which normally features a single turn. The width of the turn is dictated by the traverse speed, the available power and frequency of the generator. This creates a moving band of heat which when quenched creates the hardened surface layer. The quench ring can be either integral a following arrangement or a combination of both subject to the requirements of the application. By varying speed power etc it is possible to create a shaft which is hardened along its whole length or just in specific areas and also to harden shafts with steps in diameter or splines. It is normal when hardening round shafts to rotate the part during the process to ensure any variations due to concentricityof the coil and the component are removed.
Traverse methods also feature in the production of edge components such as paper knives, leather knives, lawnmower bottom blades, hacksaw blades etc. These types of application normally utilise a hairpin coil or a transverse flux coil which sits over the edge of the component. The component is progressed through the coil and a following spray quench consisting of nozzles or drilled blocks.
Many methods are used to provide the progressive movement through the coil and both vertical and horizontal systems are used. These normally employ a
digital encoderand programmable logic controllerfor the positional control, switching, monitoring, and setting. In all cases the speed of traverse needs to be closely controlled and consistent as variation in speed will have an effect on the depth of hardness and the hardness value achieved.
Power supplies for induction hardening vary in power from a few kilowatts to hundreds of kilowatts dependant of the size of the component to be heated and the production method employed i.e. single shot hardening, traverse hardening or submerged hardening.
In order to select the correct power supply it is first necessary to calculate the surface area of the component to be heated. Once this has been established then a variety of methods can be used to calculate the power density required, heat time and generator operating frequency. Traditionally this was done using a series of graphs, complex
empiricalcalculations and experience. Modern techniques typically utilise finite element analysisand Computer-aided manufacturingtechniques, however as with all such methods a thorough working knowledge of the induction heating process is still required.
For single shot applications the total area to be heated needs to be calculated. In the case of traverse hardening the circumference of the component is multiplied by the face width of the coil. Care must be exercised when selecting a coil face width that it is practical to construct the coil of the chosen width and that it will live at the power required for the application.
Induction heating systems for hardening are available in a variety of different operating frequencies typically from 1 KHz to 400KHz. Higher and lower frequencies are available but typically these will be used for specialist applications. The relationship between operating frequency and current penetration depth and therefore hardness depth is inversely proportional. i.e. the lower the frequency the deeper the case.
The above table is purely illustrative, good results can be obtained outside these ranges by balancing power densities, frequency and other practical considerations including cost which may influence the final selection, heat time and coil width. As well as the power density and frequency, the time the material is heated for will influence the depth to which the heat will flow by conduction. The time in the coil can be influenced by the traverse speed and the coil width, however this will also have an effect on the overall power requirement or the equipment throughput.
It can be seen from the above table that the selection of the correct equipment for any application can be extremely complex as more than one combination of power, frequency and speed can be used for a given result. However in practice many selections are immediately obvious based on previous experience and practicality.
* Induction Heating Handbook, John Davies and Peter Simpson, ISBN 0-7-084515-8
* Handbook of Induction Heating, Valery Rudnev, ISBN-10-0824708482
* Optimal Control of Induction Heating Processes, Yulia Pleshivtseva, ISBN-10-0849337542
* [http://www.inductionheating.co.uk/Induction-Heating-FAQ.htm Frequently Asked Questions About The Induction Hardening Process with examples of Induction Heating Applications]
* [http://www.namtec.co.uk The National Metals Centre offering Design, Modeling & Simulation (DMS) technologies relating to Induction Hardening processes - NAMTEC]
* [http://www.twi.co.uk Induction Hardening Centre within Research & Development of New Technologies - TWI]
Wikimedia Foundation. 2010.
Look at other dictionaries:
induction hardening — noun A process for hardening metal surfaces by induction heating followed by rapid cooling • • • Main Entry: ↑induct … Useful english dictionary
Induction hardening — Induction hardening. См. Индукционное упрочнение. (Источник: «Металлы и сплавы. Справочник.» Под редакцией Ю.П. Солнцева; НПО Профессионал , НПО Мир и семья ; Санкт Петербург, 2003 г.) … Словарь металлургических терминов
induction hardening — aukštadažnis grūdinimas statusas T sritis radioelektronika atitikmenys: angl. induction hardening vok. Hochfrequenzhärtung, f rus. высокочастотная закалка, f pranc. trempe par haute fréquence, f … Radioelektronikos terminų žodynas
induction hardening — a widely used process for the surface hardening of steel. The components are heated by means of an alternating magnetic field to a temperature within or above the transformation range followed by immediate quenching. The core of the component… … Mechanics glossary
induction hardening — Method of heating cast iron (e.g., valve seats) to approx 1700° F which hardens it to a depth of 0.05 to 0.08 inches … Dictionary of automotive terms
Induction heating — is the process of heating an electrically conducting object (usually a metal) by electromagnetic induction, where eddy currents are generated within the metal and resistance leads to Joule heating of the metal. An induction heater (for any… … Wikipedia
Induction — Most common meanings * Inductive reasoning, used in science and the scientific method * Mathematical induction, a method of proof in the field of mathematics * Electromagnetic induction in physics and engineering Other articles * Induction (play) … Wikipedia
hardening — increasing the hardness of steel by heat treatment. This normally implies heating the steel to a required temperature and quenching in a suitable medium, e.g., oil or water. age hardening case hardening cyanide hardening flame hardening induction … Mechanics glossary
induction heating — a method of heating a conducting material, as metal in a furnace, by using electromagnetic induction to establish a current in the material. [1915 20] * * * Method of raising the temperature of an electrically conductive material by subjecting it … Universalium
Case hardening — or surface hardening is the process of hardening the surface of a metal, often a low carbon steel, by infusing elements into the material s surface, forming a thin layer of a harder alloy. Case hardening is usually done after the part in question … Wikipedia